High-cycle fatigue investigations of notched Glare under different stress ratio's in various environments
- Sunil Bhat^{1}Email author and
- Sockalingam Narayanan^{2}
DOI: 10.1186/s40712-014-0003-x
© Bhat and Narayanan licensee Springer. 2014
Received: 1 March 2014
Accepted: 13 May 2014
Published: 15 October 2014
Abstract
Notched Glare 4A-3/2 laminates, comprising thin 2014-T6 aerospace aluminum alloy sheets alternately bonded with unidirectional E-glass fiber-based composite prepregs, are tested under tensile-tensile fatigue load with different stress ratio’s ranging from 0.1 to 0.5 in ambient, aqueous, and corrosive environments in high-cycle conditions. Fatigue characteristics of the laminates are found to be influenced by the operating environment and the magnitude of stress ratio. Notched plain 2014-T6 aerospace aluminum alloy specimens are also subjected to identical cyclic stress levels as in aluminum alloy layers of the laminates for comparative analysis of their fatigue behavior with those of the laminates. Retarded crack growth rates in the laminates leading to their enhanced fatigue lives and higher cyclic fracture toughness values vis-à-vis plain specimens substantiate fiber bridging effect in the laminates.
Keywords
Aqueous environment Corrosive environment Fatigue life Glare Stress ratioBackground
Glare, a fiber metal laminate (FML), consists of layers of thin and light aerospace aluminum alloy sheets that are alternately bonded and cured with composite prepregs by heat and pressure, each prepreg is built up of several resin-impregnated unidirectional fiber cloth layers laid in similar or different orientations. Besides offering gain in specific strength, Glare exhibits properties like excellent fatigue and fracture resistance, reasonably good impact strength, and high fire resistance that make it a good substitute for monolithic aluminum alloys especially in aerospace applications.
Numerous studies have so far been reported on behavior of various types of FMLs under fatigue loads of constant and variable stress ratios with most of them pertaining to tests conducted in ambient environment only. Notably, in the field of fatigue of FML under load cycles of constant stress ratio in ambient environment, Lin et al. 1991 discussed fatigue behavior in carbon- and aluminum-based FML (Care), followed by Lin and Kao (1995) investigating the effect of fiber bridging and delamination growth (Lin and Kao 1996) on crack propagation in the laminate. Guo and Wu (1998, 1999a, 1999b) presented theoretical and phenomenological models for predicting fatigue crack growth characteristics and bridging stress distribution in FML. Homan (2006) observed that fatigue crack initiation in FML depends upon the magnitude of stress in metal layer. He also investigated the effect of residual stress in fibers and in metal layers over the crack tip. Alderliesten and Homan (2006) discussed fatigue and damage tolerance issues of Glare in aircraft structures. Suiker and Fleck (2006) presented the relation between fatigue crack growth rate and remote cyclic stress with and without delaminations in a FML. Takamatsu et al. (1999) examined fatigue crack growth in Glare and checked the validity of proposed analytical models. Alderliesten (2007a) studied the propagation of fatigue cracks in aluminum layers of Glare in the presence of delaminations at aluminum-fiber interfaces. He postulated that the stress intensity parameter at the crack tip is the function of far-field opening stress and closing bridging stress in aluminum layers. An analytical model for fatigue crack propagation and transverse delamination extension using the correlation between growth rate and energy release rate of the delamination was proposed by him. The model was implemented in a numerical program, and the results were validated with the range of experimental data. Good agreement between crack growth rates, crack opening contours, and delamination shapes was obtained. Alderliesten (2007b) reviewed phenomenological, analytical, and finite element models for fatigue crack propagation prediction in Glare. Chang and Yang (2008) examined fatigue crack growth in Glare by modulating the stress intensity parameter with a bridging factor and obtained the S-N curve based on the initiation and growth life of the crack. Paris law was employed to predict crack growth rates. Shim et al. (2003) adopted a mechanistic approach to predict fatigue crack growth in Glare with the help of Paris law. Kawai and Kato (2006) examined the effects of stress ratio on off-axis fatigue behavior of Glare. They tested the coupons under different stress ratios of 0.1, 0.4 and −0.2. A fatigue damage model to account for the effect of stress ratio on crack characteristics was developed. Likewise, in the field of fatigue of FML under load cycles of variable stress ratios in ambient environment, Kawai and Hachinobe (2002) examined the effects of change in amplitude of load during the test on off-axis fatigue strength of Glare. The results of two-stress level cycles were compared with those of constant amplitude cycles. Khan et al. (2010) predicted the fatigue crack growth in Glare when subjected to variable amplitude cycles by using modified Wheeler model based on Irwin's crack tip plasticity correction and validated the theoretical results with the help of experiments.
Limited work is reported on fatigue behavior of FMLs under different stress ratios in other possible operating environments although successful attempts have been made to evaluate their properties and performance in high temperature. For instance, Rans et al. (2011) presented an analytical model to predict fatigue crack growth rate in FML operating in high temperature. The model was validated with experimental data collected in ambient conditions. da Costa et al. (2012) investigated the influence of thermal shock cycles on mechanical properties of FML. FML coupons, under cyclic load, were exposed to fast temperature transition from −50°C to +80°C. Tensile and inter-laminar shear strengths of coupons were measured after 1,000 and 2,000 cycles. No significant changes were found in micro-structure and mechanical properties of exposed coupons vis-à-vis the unexposed ones. This paper presents experimental results of series of notched Glare laminates subjected to tensile-tensile fatigue cycles with different stress ratios ranging from 0.1 to 0.5 in aqueous and corrosive environments. The laminates are tested in ambient environment as well. The stress ratio is kept constant during each test while fulfilling high-cycle conditions in the laminates. Notched plain aerospace aluminum alloy specimens are also tested under identical cyclic stress levels as those in aluminum alloy layers of the laminates for comparative analysis between them and the laminates.
Glare details
Properties of materials used in Glare
Property | Aluminum 2014-T6 alloy (al) | E-glass fiber (f) | Epoxy resin (r) |
---|---|---|---|
Modulus of elasticity (E), MPa | 72,000.0 | 71,000.0 | 3,500.0 |
Shear modulus (μ), MPa | 27,060.0 | 29,700.0 | 1,250.0 |
Poisson's ratio (υ) | 0.33 | 0.22^{*} | 0.33 |
Yield strength (Y), MPa | 372.0 | - | - |
Ultimate tensile strength, MPa | 415.0 | 3,450.0 | 60 |
Percent elongation | 8.0 | 4.8 | 4.0 |
Coefficient of thermal expansion (α), C^{−1} | 23 × 10^{− 6} | 5.0 × 10^{− 6} | 57.5 × 10^{− 6} |
Density, g/cc | 2.71 | 2.45 | 1.54 |
Plane strain fracture toughness (K_{IC}), \( \mathrm{MPa}\sqrt{\mathrm{m}} \) | 14.0 to 20.0 | 4.0 to 5.0 | 0.5 to 0.7 |
The laminate is loaded in the y direction because it demonstrates good strength and fatigue properties due to more number of c0 composites in prepregs. Since the material layers in the laminate are elastically unidentical, stress redistribution takes place in them under the action of applied stress in order to maintain same strain in all the layers. In addition, variable residual stresses are generated in the materials, during curing of the laminate, due to their different stiffness and coefficients of thermal expansions. The coefficients of thermal expansion of the laminate in longitudinal (y) direction, α_{ll}, and in transverse (x) direction, α_{tl}, are found to be equal to 19.40 × 10^{− 6} C^{−1} and 19.77 × 10^{− 6} C^{−1}, respectively, with the help of elementary formulations related to composites and laminates (Bhat and Narayanan 2014). Refer to Appendix 1. These coefficients are required to estimate the residual strain in each material layer that when superimposed with the strain developing in the laminate under maximum (max) applied tensile stress value in the fatigue cycle, σ_{y,applied,max} results in maximum induced stress value in material layer, m, as σ_{y,induced,m,max}. σ_{y,induced,m,max} therefore equals the sum of redistributed stress, σ_{y,ds,m.,max} and residual stress, σ_{y,rs,m}. Standard stress-strain constitutive equations of individual materials under plane stress condition, due to their small thickness, are employed to obtain their stiffness in the x-y plane. Classical theory is used to determine the stiffness of the laminate. Both redistributed and residual stresses in materials along the z direction are considered to be negligible. Stress state around crack tips in aluminum alloy layers further deviates from induced stress due to bridging of load over cracks towards stronger fibers, commonly referred to as fiber bridging. Fiber bridging generates closing compressive stress in aluminum alloy layers that diminishes tensile stress fields around crack tips thereby shielding them.
Theoretical aspects
Since the cracks nucleate and grow in soft aluminum alloy layers of the laminate, different forms of stress intensity parameters are found in the laminate by using stress values in aluminum alloy layers. As discussed in the ‘Glare details’ section, the redistribution of applied stress and presence of residual stress in aluminum alloy layers cause the induced stress intensity parameter, K_{induced}, to differ from the applied value, K_{applied}. Further, due to fiber bridging in the laminate, the crack tip stress intensity parameter, K_{tip}, also deviates from K_{induced}. K_{tip} is found by employing numerical or theoretical methodologies described elsewhere (Bhat and Narayanan 2014, pp. 157–160). However, in the present work, only K_{applied} and K_{induced} are used as characterizing parameters that, with the help of available experimental data, are found to be adequate to quantify the effect of fiber bridging in the laminates by comparing their fatigue behavior with that of plain aluminum alloy specimens.
- (i)
Using applied stress value in the fatigue cycle as follows:
- (ii)
Refer to Figure 2a). Using induced stress value in aluminum alloy layer as follows:
- (iii)
Refer to Figure 2b. The value of ΔK in plain aluminum alloy specimen (P) is obtained from the applied stress value only due to the absence of load redistribution and residual stress in the specimen. Since tensile residual stress in aluminum layers of the laminate does not influence its fatigue properties, maximum stress, σ_{y,applied,max}, in fatigue cycles applied over plain specimens is kept equal to σ_{y,ds,al,max} to simulate identical fatigue load in plain specimens as that in aluminum alloy layers of the laminates. ΔK in plain specimen is written as follows:
U of aluminum alloy in all the above equations is taken as 0.5 + 0.4R (Elber 1976).
Experimental method
Two-millimeter thick 2014-T6 aluminum alloy sheets were cold rolled to reduce their thickness to acceptable level that was followed by their suitable heat treatment to restore the T6 state of the aluminum alloy. Prepregs were manually prepared and stored in controlled environment prior to use. At the time of laminate fabrication, an assembly of three aluminum alloy sheets alternately reinforced with two prepregs was loaded in a hydraulic press preheated to 90°C. A pressure of 10 bar was gradually applied over the assembly. The temperature was raised to 160°C, and the assembly was cured at that temperature for 3 h. After curing, the press was cooled to room temperature followed by the release of pressure. The laminate assembly was taken out from the press and visually inspected for defects. The thickness data of all the laminates were recorded. The achieved/measured dimensional range of the laminate was as follows: t_{al} = 0.35 to 0.58 mm, d = 2.2 to 2.9 mm, l = 200 to 202 mm, and w = 50.35 to 51.35 mm. Deviations from the desired values provided in the ‘Glare details’ section, especially in laminate thickness, were attributed to (i) difficulty in maintaining precise control over thickness of aluminum alloy sheets during rolling, (ii) manual application of resin over fiber cloth during the preparation of prepregs, and (iii) effect of high temperature and bonding pressure on the dimensions of the material layers during curing of the laminate. The dimensional difference between the laminates however has not been included in the computations at Appendix 1 that are based on standard dimensions.
Mechanical properties of Glare
Property | Specimen 1 | Specimen 2 | Specimen 3 | Mean | Standard deviation |
---|---|---|---|---|---|
Yield strength (MPa) | 269.7 | 273.05 | 277.28 | 273.34 | 3.79 |
Ultimate tensile strength (MPa) | 360.3 | 365.13 | 370.62 | 365.35 | 5.163 |
Flexural strength (MPa) | 728.8 | 763.0 | 730.1 | 740.63 | 19.381 |
Shear strength (MPa) | 37.79 | 40.04 | 42.74 | 40.19 | 2.478 |
- (i)
σ_{y,applied,max} value of 75 MPa in fatigue cycle to ensure controlled crack growth rates for effective measurement and recording purpose
- (ii)
Stress ratio, R, of 0.1, 0.3, and 0.5 (all +ve). The ratio was kept constant during each test to maintain constant amplitude of load
- (iii)
Test environments namely ambient (A), aqueous (M), and corrosive (S)
Crack lengths, c, were measured. Corresponding number of cycles, N, was recorded. Crack growth rate, \( \frac{dc}{dN} \), at each crack length was computed. Values of c_{⊗} and total cycles, N_{⊗}, consumed in crack initiation at the notch tip and subsequent propagation until fracture of each laminate were noted, with N_{⊗} being the measure of fatigue life. \( \frac{dc}{dN} \) values were also obtained in the notched plain 2014-T6 aerospace aluminum alloy specimens with dimensions nearly similar as those of the laminates for comparative analysis of their fatigue behavior with those of the laminates. These specimens were subjected to tensile-tensile fatigue cycles with R of 0.1 in ambient environment alone. As discussed in the ‘Theoretical aspects’ section, the maximum stress in fatigue cycles applied over such specimens was fixed at 97.45 MPa. Refer to Appendix 1. The value of redistributed stress, σ_{y,ds,al,max}, in aluminum alloy layers of the laminate when it experiences peak applied stress of 75 MPa during the fatigue cycle is 97.45 MPa.
Results and discussion
Dimensional data and fatigue results of Glare laminates and plain aluminum alloy specimens
Series | w(mm) | d(mm) | Environment | R | c_{⊗}(mm) | N_{⊗}(cycles) |
---|---|---|---|---|---|---|
Glare laminates | ||||||
Case I | ||||||
1 | 50.55 | 2.85 | A | 0.1 | 28 | 46,328 |
2 | 50.7 | 2.5 | A | 0.5 | 34 | 115,000 |
3 | 50.8 | 2.2 | A | 0.5 | 35 | 126,270 |
4 | 50.55 | 2.55 | A | 0.5 | 15 | 58,725 |
5 | 50.5 | 2.6 | M | 0.1 | 34 | 29,163 |
6 | 50.7 | 2.48 | M | 0.3 | 35 | 22,473 |
7 | 51.35 | 2.35 | M | 0.5 | 30 | 193,503 |
8 | 51.1 | 2.9 | S | 0.1 | 13 | 5,157 |
9 | 50.35 | 2.6 | S | 0.3 | 9 | 8,671 |
Case II | ||||||
1 | 50.4 | 2.3 | A | 0.1 | 32 | 63,697 |
2 | 50.5 | 2.55 | S | 0.1 | 30 | 52,476 |
3 | 50.45 | 2.6 | A | 0.3 | 40 | 66,219 |
4 | 50.4 | 2.6 | A | 0.3 | 45 | 81,212 |
5 | 50.45 | 2.2 | S | 0.5 | 26 | 48,717 |
Plain aluminum 2014-T6 alloy specimens | ||||||
P1 | 36.3 | 1.6 | A | 0.1 | 15 | 16,575 |
P2 | 50.9 | 1.55 | A | 0.1 | 20 | 37,225 |
Case I laminates
Refer Figure 6b,c,d. (i) In ambient environment, increase in stress ratio, R, dips \( \frac{dc}{dN} \) unlike in homogeneous and some composite materials where increase in R reduces crack closure causing increase in \( \frac{dc}{dN} \). This is attributed to substantial influence of reduction in applied and induced values of cyclic stress intensity parameter due to increase in R in comparison with corresponding reduction in crack closure. Moreover, closure effects in the laminates do not appear to be dominant due to crack tip shielding caused by fiber bridging that results in minimal crack tip plasticity. Maximum \( \frac{dc}{dN} \) at R of 0.1 is 0.015 mm/cycle, while the corresponding value at R of 0.5 is 0.00347 mm/cycle. Using the applied value, the maximum fracture toughness value of laminate, ΔK_{C,applied}, is 49.74 \( \mathrm{MPa}\sqrt{\mathrm{m}} \) at R of 0.5 (U = 0.7). Likewise, using induced stress value in aluminum layers, ΔK_{C,induced} is 64.6 \( \mathrm{MPa}\sqrt{\mathrm{m}} \). (ii) In aqueous environment, increase in R again dips \( \frac{dc}{dN} \). Maximum \( \frac{dc}{dN} \) at R of 0.1 is 0.028 mm/cycle, while the corresponding value at R of 0.5 is 0.00245 mm/cycle. In comparison with ambient environment at same values of R and stress intensity parameter, \( \frac{dc}{dN} \) values are higher at lower R and lower at higher R. Laminate fracture toughness values also show an upward trend. The maximum value of ΔK_{C,applied} is 63.9 \( \mathrm{MPa}\sqrt{\mathrm{m}} \) at R of 0.1 (U = 0.54). The corresponding induced value is 83.0 \( \mathrm{MPa}\sqrt{\mathrm{m}} \). (iii) In corrosive (salt) environment, increase in R augments \( \frac{dc}{dN} \). The maximum \( \frac{dc}{dN} \) at R of 0.1 is 0.01 mm/cycle, while the corresponding value at R of 0.3 is 0.02 mm/cycle. In comparison with ambient environment at same values of R and stress intensity parameter, \( \frac{dc}{dN} \) values are more at both lower and higher values of R. In comparison with aqueous environment at same values of R and stress intensity parameter, \( \frac{dc}{dN} \) values are also more at both lower and higher values of R. Laminate fracture toughness values are much less than those in ambient and aqueous environments. The maximum value of ΔK_{C,applied} is 11.15 \( \mathrm{MPa}\sqrt{\mathrm{m}} \) at R of 0.1 (U = 0.54). The corresponding induced value is 14.48 \( \mathrm{MPa}\sqrt{\mathrm{m}} \).
Case II laminates
Refer to Figure 7b,c,d. (i) In ambient environment, increase in R dips \( \frac{dc}{dN} \), although the effect is not as high as in case I laminates. The maximum \( \frac{dc}{dN} \) at R of 0.1 is 0.01 mm/cycle, while the corresponding value at R of 0.3 is 0.0075 mm/cycle. The maximum value of ΔK_{C,applied} is 161.2 \( \mathrm{MPa}\sqrt{\mathrm{m}} \) at R of 0.3 (U = 0.62). The maximum induced value, ΔK_{C,induced}, even reaches up to 209.4 \( \mathrm{MPa}\sqrt{\mathrm{m}} \). In comparison with case I laminates in the same environment, the maximum laminate fracture toughness values are higher, and the maximum \( \frac{dc}{dN} \) values are of nearly similar magnitudes. (ii) In aqueous environment, crack did not grow in one but in all the aluminum layers, which is already discussed in case I laminate. (iii) In corrosive (salt) environment, the increase in R augments \( \frac{dc}{dN} \). The maximum \( \frac{dc}{dN} \) at R of 0.1 is 0.0028 mm/cycle, while the corresponding value at R of 0.5 is 0.0154 mm/cycle. In comparison with the ambient environment at same values of R and stress intensity parameter, \( \frac{dc}{dN} \) values are smaller at lower R but more at higher R. The data for comparison with aqueous environment are not available. The maximum value of ΔK_{C,applied} is 44.07 \( \mathrm{MPa}\sqrt{\mathrm{m}} \) at R of 0.1 (U = 0.54). The corresponding induced value is 57.26 \( \mathrm{MPa}\sqrt{\mathrm{m}} \). In comparison with case I laminate in same environment, the maximum fracture toughness values are higher, and the maximum \( \frac{dc}{dN} \) values are lesser.
Comparison between performance of laminates and plain aluminum alloy specimens
As the thickness of plain specimens is different than that of series 1 laminate, their ΔK_{C,al,∗} values corresponding to the thickness of the laminate, i.e., 2.85 mm, is determined by using Equation 8. ΔK_{IC,al,} is first obtained using ΔK_{C,al} with original specimen thickness that is followed by re-computation of ΔK_{C,al,∗} from the same equation with changed specimen thickness. The results of the plain aluminum alloy specimens are consolidated as follows:
Series P1: specimen thickness, d = 1.6 mm, w = 36.3 mm, c_{⊗} = 15 mm, \( \Delta {K}_{\mathrm{C},\mathrm{al}}=22.40\ \mathrm{MPa}\sqrt{\mathrm{m}} \) (CF = 2.179); \( \Delta {K}_{\mathrm{IC},\mathrm{al}}=14.69\ \mathrm{MPa}\sqrt{\mathrm{m}} \); for thickness of 2.85 mm, \( \Delta {K}_{\mathrm{C},\mathrm{al},\ast }=17.49\ \mathrm{MPa}\sqrt{\mathrm{m}} \).
Series P2: Specimen thickness, d = 1.55 mm, w = 50.9 mm, c_{⊗} = 20 mm \( \Delta {K}_{\mathrm{C},\mathrm{al}}=24.50\ \mathrm{MPa}\sqrt{\mathrm{m}} \) (CF = 2.065); \( \Delta {K}_{\mathrm{IC},\mathrm{al}}=15.17\ \mathrm{MPa}\sqrt{\mathrm{m}} \); for thickness of 2.85 mm, \( \Delta {K}_{\mathrm{C},\mathrm{al},\ast }=18.43\ \mathrm{MPa}\sqrt{\mathrm{m}} \)
Quasi-static K_{IC,al} values of plain specimens, equal to \( \frac{\Delta {K}_{\mathrm{IC},\mathrm{al}}}{0.9} \), are 16.32 \( \mathrm{MPa}\sqrt{\mathrm{m}} \) (series P1) and 16.85 \( \mathrm{MPa}\sqrt{\mathrm{m}} \) (series P2) that lie within the expected range of plane strain fracture toughness of 2014-T6 aluminum alloy available in Table 1. This authenticates the quality of aluminum alloy used as well as the accuracy of fatigue test equipment.
Refer to Figure 8c. To quantify the effect of fiber bridging in laminate vis-à-vis plain aluminum alloy specimen, induced cyclic stress intensity parameter values in the laminate are employed for comparison. ΔK_{C,induced} of series 1 laminate is 47.72 \( \mathrm{MPa}\sqrt{\mathrm{m}} \). On the other hand, the maximum value of ΔK_{C,al,∗} in the plain specimen (series P2) is 18.43 \( \mathrm{MPa}\sqrt{\mathrm{m}} \) which is much less than that of series 1 laminate. The values of N_{⊗} in plain specimens are 16,575 cycles (series P1) and 37,225 cycles (series P2), whereas it is 46,328 cycles for series 1 laminate. At other values of R in ambient environment, the values of N_{⊗} of the laminates are much more than those of the plain specimens. The maximum \( \frac{dc}{dN} \) of the plain specimens are 0.013 mm/cycle (series P1) and 0.083 mm/cycle (series P2) which are nearly identical or higher than that of 0.015 mm/cycle of the series 1 laminate. The values of c_{⊗} in the plain specimens are 15 mm (series P1) and 20 mm (series P2) that are also less than 28 mm in series 1 laminate. These findings convincingly confirm the phenomenon of fiber bridging in the laminate that shields the crack tips in its aluminum alloy layers, thereby retarding fatigue crack growth rates and increasing critical crack lengths leading to enhanced fatigue life and cyclic fracture toughness values of the laminate in comparison with plain aluminum alloy specimens.
Refer to Figure 8d. To compare the fracture potential of Glare laminate vis-à-vis plain aluminum alloy specimen from commercial point of view, applied cyclic stress intensity parameter values in the laminate are used in order to disregard the effects of stress redistribution and residual stress in the laminate that are missing in the plain specimens. The maximum ΔK_{C,applied} value of series 1 laminate is 36.75 \( \mathrm{MPa}\sqrt{\mathrm{m}} \) which too is higher than the maximum ΔK_{C,al,∗} of 18.43 \( \mathrm{MPa}\sqrt{\mathrm{m}} \) in plain specimens, justifiably assuming that the ΔK_{P} data of the plain specimens do not change significantly under fatigue cycles with peak stress value of 75 MPa instead of 97.45 MPa. This observation substantiates higher fatigue and fracture potential of the laminate vis-à-vis plain aluminum alloy specimens under similar load and environmental conditions.
Conclusions
- (i)
Increase in R dips fatigue crack growth rate, \( \frac{dc}{dN} \), in the laminates under ambient and aqueous environments, whereas it augments \( \frac{dc}{dN} \) in corrosive (salt) environment. The trends hold good in both case I and case II laminates.
- (ii)
Fatigue lives of laminates, N_{⊗}, change with environment. They are higher in ambient and aqueous environments and least in corrosive environment. Increase in R enhances the fatigue life in both ambient and aqueous environments in case I and in ambient environment in case II laminates due to drop in \( \frac{dc}{dN} \). In corrosive environment, N_{⊗} in case I laminates is found to increase with increase in R which is contrary to expectations since \( \frac{dc}{dN} \) increases with increase in R in such an environment. This aberration is attributed to higher crack initiation life and reduced propagation life at higher R. In case II laminates under similar environment, the results are in line with the expectations. Also, at same R in case I laminates, fatigue life in ambient environment is higher than in aqueous environment at lower R and vice versa at higher R. This is due to higher \( \frac{dc}{dN} \) values at lower R and lesser \( \frac{dc}{dN} \) values at higher R in aqueous environment in comparison with that in ambient environment. Fatigue life in ambient environment is higher than that in corrosive environment at same R in both case I and case II laminates.
- (iii)
Cyclic fracture toughness values of the laminates also change with environment. They are higher in aqueous and ambient environments and least in corrosive environment in both case I and case II laminates. In case I laminate, the values in ambient environment, in general, increase with increase in R. In aqueous environment, the values are higher at lower R and lower at higher R. In corrosive environment, the values tend to drop with increase in R. Trends in case II laminates under ambient and corrosive environments are similar to as stated for case I laminates.
- (iv)
From fatigue and fracture point of view, the laminates can be employed in aqueous environments provided that persistent or excessive exposure to water does not degrade the quality of adhesive/resin between the aluminum alloy and fiber layers leading to their separation or reduction of the strength of fibers resulting in overall property degradation of the laminate. This aspect needs to be investigated separately. But fatigue and fracture behavior of the laminates clearly deteriorates in corrosive conditions, although the results in case II are better than those in case I. Such observations go against the use of laminates in corrosive environment.
- (v)
Fatigue lives and cyclic fracture toughness of laminates are convincingly more than those of plain aluminum alloy specimens that corroborates fiber bridging in the laminates, leading to their enhanced fatigue and fracture properties.
Notations
b interfacial crack length
c mode I crack length
CF configuration factor
d thickness of laminate/plain specimen
l laminate length
t thickness of material layer
w laminate width
A ambient environment
E modulus of elasticity
FML fiber metal laminate
K stress intensity parameter
LEFM linear elastic fracture mechanics
M aqueous environment
{M} stiffness matrix
N number of fatigue cycles
R stress ratio
S corrosive environment
T temperature
U closure ratio
Y yield strength
\( \frac{dc}{dN} \) crack growth rate
1 to 8 laminate series
Symbols
α coefficient of thermal expansion
Δ cyclic value
σ normal stress
τ shear stress
υ Poisson's ratio
μ shear modulus
ε normal strain
γ shear strain
Subscripts (in plain text or in italics)
al aluminum alloy
ambient ambient temperature
applied applied value
curing curing temperature
c0 composite layer with fiber along the y direction
c90 composite layer with fiber along the x direction
ds redistributed stress
f fiber
induced induced value
lam laminate
ll value in y direction
m material layer
max maximum value
P plain aluminum alloy specimen
r resin
rs residual stress
rt residual strain
tip value at crack tip
tl value in x direction
x,y,z Cartesian coordinate system
⊗ critical value
C & IC plane stress and plane strain conditions
∗ value corresponding to laminate thickness
Declarations
Acknowledgements
Authors are grateful to the Science and Engineering Research Council, Department of Science and Technology (DST), India, for funding the project. They convey their thanks to (i) Valeth Hightech Composites Pvt. Ltd., Chennai, India, for their valuable assistance in material procurement and fabrication of the laminates and (ii) Metallurgical Services, Mumbai, India, for providing the fatigue test equipment. Support received from VIT University, Tamil Nadu, India and Galgotias University, U.P., India, during the course of this work is appreciated.
Authors’ Affiliations
References
- Alderliesten, RC. (2007a). Analytical prediction model for fatigue crack propagation and delamination growth in Glare. International Journal of Fatigue, 29(4), 628–646.View ArticleGoogle Scholar
- Alderliesten, RC. (2007b). On the available relevant approaches for fatigue crack propagation prediction in Glare. International Journal of Fatigue, 29(2), 289–304.View ArticleGoogle Scholar
- Alderliesten, RC, & Homan, JJ. (2006). Fatigue and damage tolerance issues of Glare in aircraft structures. International Journal of Fatigue, 28(10), 1116–1123.MATHView ArticleGoogle Scholar
- Bhat, S, & Narayanan, S. (2014). Quantification of fibre bridging in mode I cracked Glare without delaminations. European Journal of Mechanics A/Solids, 43(1–2), 152–170.View ArticleGoogle Scholar
- Callister, WD, Jr. (2004). Materials science and engineering: an introduction (6th ed., pp. 737–754). India: Wiley.Google Scholar
- Chang, PY, & Yang, JM. (2008). Modelling of fatigue crack growth in notched fiber metal laminates. International Journal of Fatigue, 30(12), 2165–2174.MATHView ArticleGoogle Scholar
- da Costa, AA, da Silva, DFNR, Travessa, DN, & Botelho, EC. (2012). The effect of thermal cycles on the mechanical properties of fiber-metal laminates. Materials and Design, 42(12), 434–440.View ArticleGoogle Scholar
- Elber, W. (1976). Fatigue crack growth under spectrum loads, ASTM STP 595 (pp. 236–250). Philadelphia: American Society for Testing and Materials.View ArticleGoogle Scholar
- Guo, YJ, & Wu, XR. (1998). A theoretical model for predicting fatigue crack growth rates in fiber-reinforced metal laminates. Fatigue and Fracture of Engineering Materials and Structures, 21(9), 1133–1145.View ArticleGoogle Scholar
- Guo, YJ, & Wu, XR. (1999a). A phenomenological model for predicting crack growth in fiber reinforced metal laminates under constant amplitude loading. Composites Science and Technology, 59(12), 1825–1831.View ArticleGoogle Scholar
- Guo, YJ, & Wu, XR. (1999b). Bridging stress distribution in center-cracked fiber reinforced metal laminates: modeling and experiment. Engineering Fracture Mechanics, 63(2), 147–163.MathSciNetView ArticleGoogle Scholar
- Homan, JJ. (2006). Fatigue initiation in fiber metal laminates. International Journal of Fatigue, 28(4), 366–374.View ArticleGoogle Scholar
- Irwin, GR. (1967). NRL Report 6598. Washington D.C.: Naval Research Laboratory.Google Scholar
- Kawai, M, & Hachinobe, A. (2002). Two stress level fatigue of unidirectional fiber-metal hybrid composite: GLARE 2. International Journal of Fatigue, 24(5), 567–580.View ArticleGoogle Scholar
- Kawai, M, & Kato, K. (2006). Effects of R-ratio on the off-axis fatigue behavior of unidirectional hybrid GFRP/Al laminates at room temperature. International Journal of Fatigue, 28(10), 1226–1238.MATHView ArticleGoogle Scholar
- Khan, SU, Alderliesten, RC, Rans, CD, & Benedictus, R. (2010). Application of a modified Wheeler model to predict fatigue crack growth in fiber metal laminates under variable amplitude loading. Engineering Fracture Mechanics, 77(9), 1400–1416.View ArticleGoogle Scholar
- Kumar, P. (2009). Elements of fracture mechanics (p. 91). India: McGraw-Hill.Google Scholar
- Lin, CT, & Kao, PW. (1995). Effect of fiber bridging on the fatigue crack propagation in carbon fiber-reinforced aluminum laminates. Material Science and Engineering A, 190(1–2), 65–73.View ArticleGoogle Scholar
- Lin, CT, & Kao, PW. (1996). Delamination growth and its effect on crack propagation in carbon fiber reinforced aluminum laminates under fatigue loading. Acta Materialia, 44(3), 1181–1188.View ArticleGoogle Scholar
- Lin, CT, Kao, PW, & Yang, FS. (1991). Fatigue behavior of carbon fiber-reinforced aluminum laminates. Composites, 22(2), 135–141.View ArticleGoogle Scholar
- Rans, CD, Alderliesten, RC, & Benedictus, R. (2011). Predicting the influence of temperature on fatigue crack propagation in fiber metal laminates. Engineering Fracture Mechanics, 78(10), 2193–2201.View ArticleGoogle Scholar
- Suiker, ASJ, & Fleck, NA. (2006). Modelling of fatigue crack tunneling and delamination in layered composites. Composites Part A: Applied Science and Manufacturing, 37(10), 1722–1733.View ArticleGoogle Scholar
- Shim, DJ, Alderliesten, RC, Spearing, SM, & Burianek, DA. (2003). Fatigue crack growth prediction in GLARE hybrid laminates. Composites Science and Technology, 63(12), 1759–1767.View ArticleGoogle Scholar
- Takamatsu, T, Matsumura, T, Ogura, N, Shimokawa, T, & Kakuta, Y. (1999). Fatigue crack growth properties of a GLARE3-5/4 fiber/metal laminate. Engineering Fracture Mechanics, 63(3), 253–272.View ArticleGoogle Scholar
Copyright
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.